Download presentation

Presentation is loading. Please wait.

Published byYadira Athy Modified over 2 years ago

1
Chapter 6 - 1 ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does diffusion depend on structure and temperature? Chapter 6: Diffusion

2
Chapter 6 - 2 Diffusion Diffusion - Mass transport by atomic motion Mechanisms Gases & Liquids – random (Brownian) motion Solids – vacancy diffusion or interstitial diffusion

3
Chapter 6 - 3 Interdiffusion: In an alloy, atoms tend to migrate from regions of high conc. to regions of low conc. Initially Adapted from Figs. 6.1 and 6.2, Callister & Rethwisch 4e. Diffusion After some time

4
Chapter 6 - 4 Self-diffusion: In an elemental solid, atoms also migrate. Label some atoms Diffusion A B C D After some time A B C D

5
Chapter 6 - 5 Diffusion Mechanisms Vacancy Diffusion: atoms exchange with vacancies applies to substitutional impurities atoms rate depends on: -- number of vacancies -- activation energy to exchange. increasing elapsed time

6
Chapter 6 - 6 Simulation of interdiffusion across an interface: Rate of substitutional diffusion depends on: -- vacancy concentration -- frequency of jumping (Courtesy P.M. Anderson) Diffusion Simulation This slide contains an animation that requires Quicktime and a Cinepak decompressor. Click on the message or image below to activate the animation.

7
Chapter 6 - 7 Diffusion Mechanisms Interstitial diffusion – smaller atoms can diffuse between atoms. More rapid than vacancy diffusion Adapted from Fig. 6.3 (b), Callister & Rethwisch 4e.

8
Chapter 6 - 8 Adapted from chapter-opening photograph, Chapter 6, Callister & Rethwisch 4e. (Courtesy of Surface Division, Midland-Ross.) Case Hardening: -- Diffuse carbon atoms into the host iron atoms at the surface. -- Example of interstitial diffusion is a case hardened gear. Result: The presence of C atoms makes iron (steel) harder. Processing Using Diffusion

9
Chapter 6 - 9 Doping silicon with phosphorus for n-type semiconductors: Process: 3. Result: Doped semiconductor regions. silicon Processing Using Diffusion magnified image of a computer chip 0.5 mm light regions: Si atoms light regions: Al atoms 2. Heat it. 1. Deposit P rich layers on surface. silicon Adapted from Figure 12.27, Callister & Rethwisch 4e.

10
Chapter 6 - 10 Diffusion How do we quantify the amount or rate of diffusion? J slope M = mass diffused time Measured empirically –Make thin film (membrane) of known cross-sectional area –Impose concentration gradient –Measure how fast atoms or molecules diffuse through the membrane

11
Chapter 6 - 11 Steady-State Diffusion Fick’s first law of diffusion C1C1 C2C2 x C1C1 C2C2 x1x1 x2x2 D diffusion coefficient Rate of diffusion independent of time Flux proportional to concentration gradient =

12
Chapter 6 - 12 Example: Chemical Protective Clothing (CPC) Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn. If butyl rubber gloves (0.04 cm thick) are used, what is the diffusive flux of methylene chloride through the glove? Data: –diffusion coefficient in butyl rubber: D = 110 x10 -8 cm 2 /s –surface concentrations: C 2 = 0.02 g/cm 3 C 1 = 0.44 g/cm 3

13
Chapter 6 - 13 Example (cont). glove C1C1 C2C2 skin paint remover x1x1 x2x2 Solution – assuming linear conc. gradient D = 110 x 10 -8 cm 2 /s C 2 = 0.02 g/cm 3 C 1 = 0.44 g/cm 3 x 2 – x 1 = 0.04 cm Data:

14
Chapter 6 - 14 Diffusion and Temperature Diffusion coefficient increases with increasing T D DoDo exp QdQd RT = pre-exponential [m 2 /s] = diffusion coefficient [m 2 /s] = activation energy [J/mol or eV/atom] = gas constant [8.314 J/mol-K] = absolute temperature [K] D DoDo QdQd R T

15
Chapter 6 - 15 Diffusion and Temperature Adapted from Fig. 6.7, Callister & Rethwisch 4e. (Date for Fig. 6.7 taken from E.A. Brandes and G.B. Brook (Ed.) Smithells Metals Reference Book, 7th ed., Butterworth-Heinemann, Oxford, 1992.) D has exponential dependence on T D interstitial >> D substitutional C in -Fe C in -Fe Al in Al Fe in -Fe Fe in -Fe 1000 K/T D (m 2 /s) C in -Fe C in -Fe Al in Al Fe in -Fe Fe in -Fe 0.51.01.5 10 -20 10 -14 10 -8 T( C) 15001000 600 300

16
Chapter 6 - 16 Example: At 300ºC the diffusion coefficient and activation energy for Cu in Si are D(300ºC) = 7.8 x 10 -11 m 2 /s Q d = 41.5 kJ/mol What is the diffusion coefficient at 350ºC? transform data D Temp = T ln D 1/T

17
Chapter 6 - 17 Example (cont.) T 1 = 273 + 300 = 573 K T 2 = 273 + 350 = 623 K D 2 = 15.7 x 10 -11 m 2 /s

18
Chapter 6 - 18 Non-steady State Diffusion The concentration of diffusing species is a function of both time and position C = C(x,t) In this case Fick’s Second Law is used Fick’s Second Law

19
Chapter 6 - VMSE: Screenshot of Diffusion Computations & Data Plots 19

20
Chapter 6 - 20 Non-steady State Diffusion Adapted from Fig. 6.5, Callister & Rethwisch 4e. B.C. at t = 0, C = C o for 0 x at t > 0, C = C S for x = 0 (constant surface conc.) C = C o for x = Copper diffuses into a bar of aluminum. pre-existing conc., C o of copper atoms Surface conc., C of Cu atoms bar s C s

21
Chapter 6 - 21 Solution: C(x,t) = Conc. at point x at time t erf (z) = error function erf(z) values are given in Table 6.1 CSCS CoCo C(x,t)C(x,t) Adapted from Fig. 6.5, Callister & Rethwisch 4e.

22
Chapter 6 - 22 Non-steady State Diffusion Sample Problem: An FCC iron-carbon alloy initially containing 0.20 wt% C is carburized at an elevated temperature and in an atmosphere that gives a surface carbon concentration constant at 1.0 wt%. If after 49.5 h the concentration of carbon is 0.35 wt% at a position 4.0 mm below the surface, determine the temperature at which the treatment was carried out. Solution: use Eqn. 6.5

23
Chapter 6 - 23 Solution (cont.): –t = 49.5 h x = 4 x 10 -3 m –C x = 0.35 wt%C s = 1.0 wt% –C o = 0.20 wt% erf(z) = 0.8125

24
Chapter 6 - 24 Solution (cont.): We must now determine from Table 6.1 the value of z for which the error function is 0.8125. An interpolation is necessary as follows zerf(z) 0.900.7970 z0.8125 0.950.8209 z 0.93 Now solve for D

25
Chapter 6 - 25 To solve for the temperature at which D has the above value, we use a rearranged form of Equation (6.9a); from Table 6.2, for diffusion of C in FCC Fe D o = 2.3 x 10 -5 m 2 /s Q d = 148,000 J/mol Solution (cont.): T = 1300 K = 1027°C

26
Chapter 6 - 26 Example: Chemical Protective Clothing (CPC) Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn. If butyl rubber gloves (0.04 cm thick) are used, what is the breakthrough time (t b ), i.e., how long could the gloves be used before methylene chloride reaches the hand? Data –diffusion coefficient in butyl rubber: D = 110 x10 -8 cm 2 /s

27
Chapter 6 - 27 CPC Example (cont.) Time required for breakthrough ca. 4 min glove C1C1 C2C2 skin paint remover x1x1 x2x2 Solution – assuming linear conc. gradient Equation from online CPC Case Study 5 at the Student Companion Site for Callister & Rethwisch 4e (www.wiley.com/ college/callister) D = 110 x 10 -8 cm 2 /s Breakthrough time = t b

28
Chapter 6 - 28 Diffusion FASTER for... open crystal structures materials w/secondary bonding smaller diffusing atoms lower density materials Diffusion SLOWER for... close-packed structures materials w/covalent bonding larger diffusing atoms higher density materials Summary

29
Chapter 6 - 29 Core Problems: Self-help Problems: ANNOUNCEMENTS Reading:

Similar presentations

OK

ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases?

ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases?

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google